2012. 2012. NEW WET WHITE TANNING AGENTS AND TEHNOLOGY. Marian Crudu, Viorica Deselnicu, Ioannis Ioannidis, Andra Crudu Leather and Footwear Research Institute, Ion Minulescu 93, Bucharest, Romania, firstname.lastname@example.org. 3. RESULTS AND DISCUSSIONS
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
NEW WET WHITE TANNING AGENTS AND TEHNOLOGY
Marian Crudu, Viorica Deselnicu, Ioannis Ioannidis, Andra Crudu
Leather and Footwear Research Institute, Ion Minulescu 93, Bucharest, Romania, email@example.com
3. RESULTS AND DISCUSSIONS
The results of chemical analysis carried out for the novel tanning agents’ solution and powder form are reported in Table 2.
Table 2 - Chemical analysis of the Tanning agents
The evaluation new tanning agents’, and in particular topographic distribution – mapping - of the metal species, was obtained by means of scanning electron microscopic (SEM) and energy dispersive X-ray (EDAX) analyses (Figure 2).
New Wet-White leathers characterization and evaluation
Shrinkage temperature values determined for the different new tanning agent variants ranged from 68-820C, whereas wet white leathers were successfully processed through the subsequent mechanical operations of splitting – easily grain, middle and bottom split were obtained, as well as shaving, as demonstrated with the photographic image of Figure 3.
Good hydrothermal stability of the prototype leathers was confirmed with measurements undertaken using the Micro-Hot table device, with Ts=70-80oC, as shown in Figure 3.
Another confirmation of the thermal behavior of the new semi-wet type of leather tanned with white pre-tanning agents was obtained by using DSC analysis (differential scanning calorimetric dynamic analysis). A typical example of the thermographs recorded for samples taken from the prototype wet-white leathers tanned with the new Ti-Al based tanning agents is shown in the Figure 4.
Exploring the valorisation of solid Titanium metallurgic end wastes, as a low cost raw material has yielded new tanning agents for the replacement of Cr(III) tanning salts, a hitherto unthinkable or non technically feasible mission. In turn, as demonstrated here it is plausible to:
- increase of eco-efficiency in the leather manufacturing sector by making use of solid wastes, which cannot be recycled in the industry that generated them;
- total or partial replacement of chromium salts in the tanning process with cheap to produce and easy to apply in rapid full substance bovine leather manufacture, that, in turn required minimum process rationalisation or modification; moreover, the new mineral tanning agents are free of restricted or regulated metals Cr, Pb, Cd, Hg and Ni
- increase in articles diversity
The experimental results obtained so far in pretanning trials, are a clear witness that it is now possible at pilot scale to produce full substance bovine wet white with the desired smooth grain, that possesses the minimum hydrothermal stability for subsequent mechanical processing and further R&D ought to be carried out aiming at:
- improving the methods of waste processing to make them more efficient;
- a complete survey of environmental impact and LCIA of the products, effluent and waste generated
- obtaining quantitative yield and costing data from large scale lots
- the diversification and rendering more efficient the tanning materials, application processes, and wet-white leather semi-processed commodity products.
Figure 2.Mappingof scanning electron microscopic (SEM) and energy dispersive X-ray (EDAX) analyses
The main classification criterion for titanium wastes was their contaminant level (Buzatu M., 1994). The highest contaminant level in titanium wastes and titanium alloys is in cuttings resulting from the mechanical processing of ingots and cast articles
Basic metal composition of the Titanium wastes (filings) used as raw materials for the production of the new Ti (III) tanning agents is given in Table 1.
Table 1 - Chemical composition
Figure 3. Hydrothermal stability using the Micro-Hot table device
The Aluminum salt used was Al2(SO4)3 . 18 H2O (15.3% Al2O3, 8.55% Al)
The schematic outline of the synthetic pathway designed and applied for the generation of the mixed new tanning agents based on Titanium and Aluminum is shown in Figure 1( Crudu M. et. al.,, 2008, 2009 )
This work has been financed by the European Fund for Regional Development and the Romanian Government in the framework of Sectoral Operational Programme under the project INNOVA-LEATHER: «Innovative technologies for leather sector increasing technological competitiveness by RDI, quality of life and environmental protection» – contract POS CCE-AXA 2-O 2.1.2 nr. 242/20.09.2010 ID 638 COD SMIS – CSNR 12579
Figure 4. DSC analysis (obtained in nitrogen flow) for the pickled hides
The evaluation of the modification of collagen by new tanning agents’, and in particular topographic distribution – mapping - of the metal species in the prototype leathers, was obtained by means of scanning electron microscopy (SEM) and energy dispersive X-ray analysis (EDAX). These are most appropriate methods for the characterization of surfaces and the results obtained confirm all previous assumptions about metal tanning agents uniform penetration and distribution, as well as provide semi-quantitative data of the mineral species topographic mapping (Figure 5).
Mineral species topographic SEM – image of grain
Mapping split of wet white leather
Figure 1. Chemical synthesis pathway
for obtaining the new tanning agents
based on Ti and Al
INTERNATIONAL CONFERENCE ON
ADVANCED MATERIALS AND SYSTEMS
27-29 September, Bucharest, Romania